| %CaO | %BaO | %AlO3/2 | T g (degC) | T  x  (degC) | T  x  - T g (degC) |
| 47.5 | 5    | 47.5    | 776        | 923          | 147                |
| 45   | 7.5  | 47.5    | 761        | 905          | 144                |
| 42.5 | 10   | 47.5    | 754        | 880          | 126                |
| 45   | 5    | 50      | 783        | 921          | 138                |
| 42.5 | 7.5  | 50      | 767        | 929          | 162                |
| 40   | 10   | 50      | 776        | 910          | 134                |
| 42.5 | 5    | 52.5    | 805        | 936          | 131                |
| 40   | 7.5  | 52.5    | 802        | 936          | 134                |
| 44.2 | 0    | 55.8    | 842        | 967          | 125                |
| 42.4 | 1.8  | 55.8    | 845        | 971          | 126                |
| 40.5 | 3.7  | 55.8    | 831        | 961          | 130                |
| 40   | 5    | 55      | 823        | 960          | 137                |
| 38.7 | 5.5  | 55.8    | 830        | 951          | 121                |
| 36.8 | 7.4  | 55.8    | 810        | 936          | 126                |
| 37.5 | 7.5  | 55      | 825        | 945          | 120                |
| 35   | 10   | 55      | 818        | 927          | 109                |
| 37.5 | 5    | 57.5    | 848        | 961          | 113                |
| 35   | 7.5  | 57.5    | 841        | 947          | 106                |

Caption: Thermal properties of CaBa aluminate glasses

You are provided with a table from a material science paper. Here are JSON templates for two types of numeric cells: "Other" and "Glass_Compound_Amount":
{"value": "xx", "type": "Other"}
{"value": "xx", "type": "Glass_Compound_Amount", "constituent": "xx", "unit": "xx", "material": "xx"}

Please describe all numeric cells in the above table following the JSON templates (proceeding by row in a left-right, top-down direction). For each cell, output one JSON description per line. For any unanswerable attributes in the templates, set their value to the placeholder "xx".

Cell Description:
{"value": "47.5", "type": "Glass_Compound_Amount", "constituent": "CaO", "unit": "mol", "material": "xx"}
{"value": "5", "type": "Glass_Compound_Amount", "constituent": "BaO", "unit": "mol", "material": "xx"}
{"value": "47.5", "type": "Glass_Compound_Amount", "constituent": "AlO3/2", "unit": "mol", "material": "xx"}
{"value": "776", "type": "Other"}
{"value": "923", "type": "Other"}
{"value": "147", "type": "Other"}
{"value": "45", "type": "Glass_Compound_Amount", "constituent": "CaO", "unit": "mol", "material": "xx"}
{"value": "7.5", "type": "Glass_Compound_Amount", "constituent": "BaO", "unit": "mol", "material": "xx"}
{"value": "47.5", "type": "Glass_Compound_Amount", "constituent": "AlO3/2", "unit": "mol", "material": "xx"}
{"value": "761", "type": "Other"}
{"value": "905", "type": "Other"}
{"value": "144", "type": "Other"}
{"value": "42.5", "type": "Glass_Compound_Amount", "constituent": "CaO", "unit": "mol", "material": "xx"}
{"value": "10", "type": "Glass_Compound_Amount", "constituent": "BaO", "unit": "mol", "material": "xx"}
{"value": "47.5", "type": "Glass_Compound_Amount", "constituent": "AlO3/2", "unit": "mol", "material": "xx"}
{"value": "754", "type": "Other"}
{"value": "880", "type": "Other"}
{"value": "126", "type": "Other"}
{"value": "45", "type": "Glass_Compound_Amount", "constituent": "CaO", "unit": "mol", "material": "xx"}
{"value": "5", "type": "Glass_Compound_Amount", "constituent": "BaO", "unit": "mol", "material": "xx"}
{"value": "50", "type": "Glass_Compound_Amount", "constituent": "AlO3/2", "unit": "mol", "material": "xx"}
{"value": "783", "type": "Other"}
{"value": "921", "type": "Other"}
{"value": "138", "type": "Other"}
{"value": "42.5", "type": "Glass_Compound_Amount", "constituent": "CaO", "unit": "mol", "material": "xx"}
{"value": "7.5", "type": "Glass_Compound_Amount", "constituent": "BaO", "unit": "mol", "material": "xx"}
{"value": "50", "type": "Glass_Compound_Amount", "constituent": "AlO3/2", "unit": "mol", "material": "xx"}
{"value": "767", "type": "Other"}
{"value": "929", "type": "Other"}
{"value": "162", "type": "Other"}
{"value": "40", "type": "Glass_Compound_Amount", "constituent": "CaO", "unit": "mol", "material": "xx"}
{"value": "10", "type": "Glass_Compound_Amount", "constituent": "BaO", "unit": "mol", "material": "xx"}
{"value": "50", "type": "Glass_Compound_Amount", "constituent": "AlO3/2", "unit": "mol", "material": "xx"}
{"value": "776", "type": "Other"}
{"value": "910", "type": "Other"}
{"value": "134", "type": "Other"}
{"value": "42.5", "type": "Glass_Compound_Amount", "constituent": "CaO", "unit": "mol", "material": "xx"}
{"value": "5", "type": "Glass_Compound_Amount", "constituent": "BaO", "unit": "mol", "material": "xx"}
{"value": "52.5", "type": "Glass_Compound_Amount", "constituent": "AlO3/2", "unit": "mol", "material": "xx"}
{"value": "805", "type": "Other"}
{"value": "936", "type": "Other"}
{"value": "131", "type": "Other"}
{"value": "40", "type": "Glass_Compound_Amount", "constituent": "CaO", "unit": "mol", "material": "xx"}
{"value": "7.5", "type": "Glass_Compound_Amount", "constituent": "BaO", "unit": "mol", "material": "xx"}
{"value": "52.5", "type": "Glass_Compound_Amount", "constituent": "AlO3/2", "unit": "mol", "material": "xx"}
{"value": "802", "type": "Other"}
{"value": "936", "type": "Other"}
{"value": "134", "type": "Other"}
{"value": "44.2", "type": "Glass_Compound_Amount", "constituent": "CaO", "unit": "mol", "material": "xx"}
{"value": "0", "type": "Other"}
{"value": "55.8", "type": "Glass_Compound_Amount", "constituent": "AlO3/2", "unit": "mol", "material": "xx"}
{"value": "842", "type": "Other"}
{"value": "967", "type": "Other"}
{"value": "125", "type": "Other"}
{"value": "42.4", "type": "Glass_Compound_Amount", "constituent": "CaO", "unit": "mol", "material": "xx"}
{"value": "1.8", "type": "Glass_Compound_Amount", "constituent": "BaO", "unit": "mol", "material": "xx"}
{"value": "55.8", "type": "Glass_Compound_Amount", "constituent": "AlO3/2", "unit": "mol", "material": "xx"}
{"value": "845", "type": "Other"}
{"value": "971", "type": "Other"}
{"value": "126", "type": "Other"}
{"value": "40.5", "type": "Glass_Compound_Amount", "constituent": "CaO", "unit": "mol", "material": "xx"}
{"value": "3.7", "type": "Glass_Compound_Amount", "constituent": "BaO", "unit": "mol", "material": "xx"}
{"value": "55.8", "type": "Glass_Compound_Amount", "constituent": "AlO3/2", "unit": "mol", "material": "xx"}
{"value": "831", "type": "Other"}
{"value": "961", "type": "Other"}
{"value": "130", "type": "Other"}
{"value": "40", "type": "Glass_Compound_Amount", "constituent": "CaO", "unit": "mol", "material": "xx"}
{"value": "5", "type": "Glass_Compound_Amount", "constituent": "BaO", "unit": "mol", "material": "xx"}
{"value": "55", "type": "Glass_Compound_Amount", "constituent": "AlO3/2", "unit": "mol", "material": "xx"}
{"value": "823", "type": "Other"}
{"value": "960", "type": "Other"}
{"value": "137", "type": "Other"}
{"value": "38.7", "type": "Glass_Compound_Amount", "constituent": "CaO", "unit": "mol", "material": "xx"}
{"value": "5.5", "type": "Glass_Compound_Amount", "constituent": "BaO", "unit": "mol", "material": "xx"}
{"value": "55.8", "type": "Glass_Compound_Amount", "constituent": "AlO3/2", "unit": "mol", "material": "xx"}
{"value": "830", "type": "Other"}
{"value": "951", "type": "Other"}
{"value": "121", "type": "Other"}
{"value": "36.8", "type": "Glass_Compound_Amount", "constituent": "CaO", "unit": "mol", "material": "xx"}
{"value": "7.4", "type": "Glass_Compound_Amount", "constituent": "BaO", "unit": "mol", "material": "xx"}
{"value": "55.8", "type": "Glass_Compound_Amount", "constituent": "AlO3/2", "unit": "mol", "material": "xx"}
{"value": "810", "type": "Other"}
{"value": "936", "type": "Other"}
{"value": "126", "type": "Other"}
{"value": "37.5", "type": "Glass_Compound_Amount", "constituent": "CaO", "unit": "mol", "material": "xx"}
{"value": "7.5", "type": "Glass_Compound_Amount", "constituent": "BaO", "unit": "mol", "material": "xx"}
{"value": "55", "type": "Glass_Compound_Amount", "constituent": "AlO3/2", "unit": "mol", "material": "xx"}
{"value": "825", "type": "Other"}
{"value": "945", "type": "Other"}
{"value": "120", "type": "Other"}
{"value": "35", "type": "Glass_Compound_Amount", "constituent": "CaO", "unit": "mol", "material": "xx"}
{"value": "10", "type": "Glass_Compound_Amount", "constituent": "BaO", "unit": "mol", "material": "xx"}
{"value": "55", "type": "Glass_Compound_Amount", "constituent": "AlO3/2", "unit": "mol", "material": "xx"}
{"value": "818", "type": "Other"}
{"value": "927", "type": "Other"}
{"value": "109", "type": "Other"}
{"value": "37.5", "type": "Glass_Compound_Amount", "constituent": "CaO", "unit": "mol", "material": "xx"}
{"value": "5", "type": "Glass_Compound_Amount", "constituent": "BaO", "unit": "mol", "material": "xx"}
{"value": "57.5", "type": "Glass_Compound_Amount", "constituent": "AlO3/2", "unit": "mol", "material": "xx"}
{"value": "848", "type": "Other"}
{"value": "961", "type": "Other"}
{"value": "113", "type": "Other"}
{"value": "35", "type": "Glass_Compound_Amount", "constituent": "CaO", "unit": "mol", "material": "xx"}
{"value": "7.5", "type": "Glass_Compound_Amount", "constituent": "BaO", "unit": "mol", "material": "xx"}
{"value": "57.5", "type": "Glass_Compound_Amount", "constituent": "AlO3/2", "unit": "mol", "material": "xx"}
{"value": "841", "type": "Other"}
{"value": "947", "type": "Other"}
{"value": "106", "type": "Other"}